Table 32. Continued. 



Alloy 



Ni 



C 



Mn 



Fe 



S 



Si 



Cu 



Cr 



Ti 



Mo 



Cb 



Other 



Source 



Ni-Cr 65-35 



65.0 



- 



- 



- 



- 



- 



- 



35.0 



- 



- 



- 



- 



INCO (3) 



Ni-Cr 75 



78.0 



- 



- 



- 



- 



- 



- 



20.0 



- 



- 



- 



- 



INCO(3) 



Ni-Cr 80-20 



80.0 



- 



- 



- 



- 



- 



- 



20.0 



- 



- 



- 



- 



INCO (3) 



Ni-Si"D" 



86.0 



- 



- 



- 



- 



10.0 



3.0 



- 



- 



- 



- 



- 



INCO (3) 



Filler metal 62 



73.5 



0.04 



0.20 



7.50 



0.007 



0.30 



0.03 



16.0 



- 



- 



2.3 



- 



CEL (4) 



Filler metal 65 



42.0 



0.03 



0.80 



30.0 



0.008 



0.30 



1.70 



21.0 



0.90 



3.0 



- 



- 



CEL (4) 



Filler metal 69 



72.8 



0.04 



0.70 



6.80 



0.007 



0.30 



0.05 



15.2 



2.40 



- 



0.85 



0.80 Al 



CEL (4) 



Filler metal 82 



72.0 



0.02 



3.00 



1.00 



0.007 



0.20 



0.02 



20.0 



0.5 



- 



2.5 



- 



CEL (4) 



Electrode 132 



74.0 



0.05 



0.75 



8.50 



0.005 



0.20 



0.10 



14.0 



- 



- 



2.0 



0.1 Ce 



CEL (4) 



Electrode 135 



38.0 



0.05 



0.50 



31.0 



0.008 



0.40 



1.80 



19.0 



- 



5.5 



1.0 



- 



CEL (4) 



Electrode 1 38 



38.0 



0.16 



1.90 



27.0 



0.008 



0.40 



0.40 



28.0 



- 



3.60 



- 



1.0 w 



CEL (4) 



Electrode 182 



68.0 



0.05 



7.50 



7.50 



0.005 



0.60 



0.10 



14.0 



- 



- 



2.0 



0.1 Ce 



CEL (4) 



Filler metal 718 



52.5 



0.04 



0.20 



18.0 



0.007 



0.20 



0.10 



19.0 



0.80 



3.0 



- 



" 



CEL (4) 



Numbers refer to references at end of report. 

 Wire rope and bolts. 

 Wire rope. 



109 



